##############################################################################
###      FullProf-generated CIF output file  (version: December 2016)      ###
###      Template of CIF submission form for structure report              ###
##############################################################################
 
# This file has been generated using FullProf.2k taking one example of 
# structure report provided by Acta Cryst. It is given as a 'template' with 
# filled structural items. Many other items are left unfilled and it is the  
# responsibility of the user to properly fill or suppress them. In principle 
# all question marks '?' should be replaced by the appropriate text or 
# numerical value depending on the kind of CIF item. 
# See the document: cif_core.dic (URL: http://www.iucr.org) for details. 
 
# Please notify any error or suggestion to: 
#           Juan Rodriguez-Carvajal (jrc@ill.eu)
# Improvements will be progressively added as needed.
 
#=============================================================================
 data_global
#=============================================================================
 
# PROCESSING SUMMARY (IUCr Office Use Only)
 
_journal_data_validation_number      ?
 
_journal_date_recd_electronic        ?
_journal_date_to_coeditor            ?
_journal_date_from_coeditor          ?
_journal_date_accepted               ?
_journal_date_printers_first         ?
_journal_date_printers_final         ?
_journal_date_proofs_out             ?
_journal_date_proofs_in              ?
_journal_coeditor_name               ?
_journal_coeditor_code               ?
_journal_coeditor_notes
; ?
;
_journal_techeditor_code             ?
_journal_techeditor_notes
; ?
;
_journal_coden_ASTM                  ?
_journal_name_full                   ?
_journal_year                        ?
_journal_volume                      ?
_journal_issue                       ?
_journal_page_first                  ?
_journal_page_last                   ?
_journal_paper_category              ?
_journal_suppl_publ_number           ?
_journal_suppl_publ_pages            ?
 
#=============================================================================
 
# 1. SUBMISSION DETAILS
 
_publ_contact_author_name            ?  # Name of author for correspondence
_publ_contact_author_address            # Address of author for correspondence
; ?
;
_publ_contact_author_email           ?
_publ_contact_author_fax             ?
_publ_contact_author_phone           ?
 
_publ_contact_letter
; ?
;
 
_publ_requested_journal              ?
_publ_requested_coeditor_name        ?
_publ_requested_category             ?   # Acta C: one of CI/CM/CO/FI/FM/FO
 
 
# Definition of non standard CIF items (Reliability indices used in FULLPROF) 
 
loop_ 
_publ_manuscript_incl_extra_item
_publ_manuscript_incl_extra_info
_publ_manuscript_incl_extra_defn
#      Name                               Explanation                 Standard?
#     ------                              -----------                 ---------
 '_pd_proc_ls_prof_cR_factor'    'Prof. R-factor CORRECTED for background'   no
 '_pd_proc_ls_prof_cwR_factor'   'wProf.R-factor CORRECTED for background'   no
 '_pd_proc_ls_prof_cwR_expected' 'wProf.Expected CORRECTED for background'   no
 '_pd_proc_ls_prof_chi2'         'Chi-square for all considered points'      no
 '_pd_proc_ls_prof_echi2'        'Chi-2 for points with Bragg contribution'  no
#=============================================================================
 
# 3. TITLE AND AUTHOR LIST
 
_publ_section_title
; ' BiFe0.7Sc0.3O3 as prepared'
;
_publ_section_title_footnote
;
;
 
# The loop structure below should contain the names and addresses of all 
# authors, in the required order of publication. Repeat as necessary.
 
loop_
    _publ_author_name
    _publ_author_footnote
    _publ_author_address
?                                   #<--'Last name, first name' 
; ?
;
; ?
;
 
#=============================================================================
 
# 4. TEXT
 
_publ_section_synopsis
;  ?
;
_publ_section_abstract
; ?
;          
_publ_section_comment
; ?
;
_publ_section_exptl_prep      # Details of the preparation of the sample(s)
                              # should be given here. 
; ?
;
_publ_section_exptl_refinement
; ?
;
_publ_section_references
; ?
;
_publ_section_figure_captions
; ?
;
_publ_section_acknowledgements
; ?
;
 
#=============================================================================
 
#=============================================================================
# If more than one structure is reported, the remaining sections should be 
# completed per structure. For each data set, replace the '?' in the
# data_? line below by a unique identifier.
 
data_nuclear
 
#=============================================================================
 
# 5. CHEMICAL DATA
 
_chemical_name_systematic
; ?
;
_chemical_name_common             ?
_chemical_formula_moiety          'Bi16 Fe11.20 O48 Sc4.80' 
_chemical_formula_structural      ?
_chemical_formula_analytical      ?
_chemical_formula_iupac           ?
_chemical_formula_sum             'Bi16 Fe11.20 O48 Sc4.80'
_chemical_formula_weight          4953.01
_chemical_melting_point           ?
_chemical_compound_source         ?       # for minerals and 
                                          # natural products
 
loop_
    _atom_type_symbol               
    _atom_type_scat_length_neutron      
    _atom_type_scat_source          
BI     0.85320 V.F._Sears_Neutron_News_3_26_(1992)
FE     0.94500 V.F._Sears_Neutron_News_3_26_(1992)
SC     1.22900 V.F._Sears_Neutron_News_3_26_(1992)
O      0.58030 V.F._Sears_Neutron_News_3_26_(1992)
 
#=============================================================================
 
# 6. POWDER SPECIMEN AND CRYSTAL DATA
 
_symmetry_cell_setting                   orthorhombic
_symmetry_space_group_name_H-M           'P n m a'
_symmetry_space_group_name_Hall          '-P 2ac 2n'
_symmetry_Int_Tables_number              62

loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -x+1/2,-y,z+1/2
 3   -x,y+1/2,-z
 4   x+1/2,-y+1/2,-z+1/2
 5   -x,-y,-z
 6   x+1/2,y,-z+1/2
 7   x,-y+1/2,z
 8   -x+1/2,y+1/2,z+1/2

_cell_length_a                           5.6605(2)
_cell_length_b                           15.7832(5)
_cell_length_c                           11.3751(4)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        90
_cell_volume                             1016.26(6)


_cell_formula_units_Z                    1
_cell_measurement_temperature            300
_cell_special_details
; ?
;

_exptl_crystal_density_diffrn            8.0929
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            ?
_exptl_crystal_F_000                     709

_pd_spec_size_axial                      ?
_pd_spec_size_equat                      ?
_pd_spec_size_thick                      ?
_pd_spec_mounting                        ?
_pd_spec_mount_mode                      ?
_pd_spec_shape                           ?
_pd_char_particle_morphology             ?
_pd_char_colour                          brown
_pd_prep_cool_rate                       ?
_pd_prep_pressure                        ?
_pd_prep_temperature                     ?

_exptl_absorpt_coefficient_mu            0
_exptl_absorpt_correction_type           ?
_exptl_absorpt_process_details           ?
_exptl_absorpt_correction_T_min          ?
_exptl_absorpt_correction_T_max          ?
loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 ? ? ? ?
 
#=============================================================================
 
# 7. EXPERIMENTAL DATA
 
_exptl_special_details
; ?
;
 
# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.
 
_pd_instr_location
; ?
;
_pd_calibration_special_details           # description of the method used
                                          # to calibrate the instrument
; ?
;
 
_diffrn_ambient_temperature          300
_diffrn_source           'spallation source'
_diffrn_source_target     ?  # Put here the type of target 
_diffrn_radiation_type   neutron 
_diffrn_source_type       ?  # Put here the diffractometer and site 
 
_diffrn_radiation_monochromator      ?
_diffrn_measurement_device_type      'WISH beamline, ISIS'
_diffrn_measurement_method           ?
_diffrn_detector_area_resol_mean     ? 
_diffrn_detector                     ?
_diffrn_detector_type                ? # make or model of detector
_pd_meas_scan_method      'tof'   # options are 'step', 'cont',
                              # 'tof', 'fixed' or
                              # 'disp' (= dispersive)
_pd_meas_special_details
;  ?
;
 
#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.
 
_pd_meas_number_of_points         4122
_pd_meas_2theta_range_min         7463.46338
_pd_meas_2theta_range_max         109083.48438
_pd_meas_2theta_range_inc         25.158762
 
# The following three items are used for time-of-flight measurements only.
 
_pd_instr_dist_src/spec           ?
_pd_instr_dist_spec/detc          ?
_pd_meas_2theta_fixed             121.6600
 
#=============================================================================
 
# 8. REFINEMENT DATA
 
_refine_special_details
; ?
;
 
# Use the next field to give any special details about the fitting of the
# powder pattern.
 
_pd_proc_ls_special_details
; ?
;
 
# The next three items are given as text.
 
_pd_proc_ls_profile_function      ?
_pd_proc_ls_background_function   ?
_pd_proc_ls_pref_orient_corr
; ?
;
 
#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard
 
_pd_proc_ls_prof_R_factor                4.2762
_pd_proc_ls_prof_wR_factor               4.9997
_pd_proc_ls_prof_wR_expected             1.5066
 
#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above
 
_pd_proc_ls_prof_cR_factor               13.0246
_pd_proc_ls_prof_cwR_factor               9.8563
_pd_proc_ls_prof_cwR_expected             2.9702
 
#  The following items are not in the CIF standard, but are defined above
 
_pd_proc_ls_prof_chi2                11.0119
_pd_proc_ls_prof_echi2               11.0598
 
#  Items related to LS refinement
 
_refine_ls_R_I_factor                 5.1535
_refine_ls_number_reflns                  3391
_refine_ls_number_parameters               109
_refine_ls_number_restraints                 0
 
_pd_block_diffractogram_id        ?  # The id used for the block containing
                                     # the powder pattern profile (section 11)
 
# Give appropriate details in the next two text fields.
 
_pd_proc_info_excluded_regions    ?
_pd_proc_info_data_reduction      ?
 
# The following items are used to identify the programs used.
 
_computing_data_collection           ?
_computing_structure_solution        ?
_computing_structure_refinement      FULLPROF
_computing_molecular_graphics        ?
_computing_publication_material      ?
 
#=============================================================================
 
# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS
 
loop_
    _atom_site_label
    _atom_site_fract_x
    _atom_site_fract_y
    _atom_site_fract_z
    _atom_site_U_iso_or_equiv
    _atom_site_occupancy
    _atom_site_adp_type
    _atom_site_type_symbol
 Bi1  0.170(4)  0.25000  0.6242(17)  0.0228(19)  1.00000 Uiso Bi    
 Bi2  0.293(4)  0.25000  0.1336(17)  0.0228(19)  1.00000 Uiso Bi    
 Bi3  0.2868(17) -0.0117(7)  0.1206(11)  0.0228(19)  1.00000 Uiso Bi    
 Fe1  0.7658(20)  0.6222(6)  0.1227(11)  0.0212(12)  0.70000 Uiso Fe    
 Sc1  0.7658(20)  0.6222(6)  0.1227(11)  0.0212(12)  0.30000 Uiso Sc    
 Fe2  0.756(2)  0.1344(5)  0.1214(11)  0.0212(12)  0.70000 Uiso Fe    
 Sc2  0.756(2)  0.1344(5)  0.1214(11)  0.0212(12)  0.30000 Uiso Sc    
 O1  0.038(2)  0.6142(9)  0.0110(17)  0.0177(16)  1.00000 Uiso O     
 O2  0.022(3)  0.5920(9)  0.507(2)  0.0177(16)  1.00000 Uiso O     
 O3  0.532(4)  0.6557(11)  0.7625(18)  0.0177(16)  1.00000 Uiso O     
 O4  0.554(3)  0.1371(10)  0.7737(16)  0.0177(16)  1.00000 Uiso O     
 O5  0.816(5)  0.25000  0.605(3)  0.0177(16)  1.00000 Uiso O     
 O6  0.684(5)  0.25000  0.091(3)  0.0177(16)  1.00000 Uiso O     
 O7  0.727(2) -0.0020(11)  0.1674(11)  0.0177(16)  1.00000 Uiso O     
 
# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.
 
#=============================================================================
 
# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 
 
_geom_special_details                ?
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Bi1 O1 . 2_565 3.00(2) ?
  Bi1 O1 . 8_545 3.00(2) ?
  Bi1 O4 . 4_456 2.23(2) ?
  Bi1 O4 . 6_456 2.23(2) ?
  Bi1 O5 . 1_455 2.02(4) ?
  Bi1 O6 . 4_455 2.45(4) ?
  Bi2 O2 . 2_564 3.07(2) ?
  Bi2 O2 . 8_544 3.07(2) ?
  Bi2 O3 . 2_564 2.78(3) ?
  Bi2 O3 . 3_646 2.13(3) ?
  Bi2 O3 . 5_666 2.13(3) ?
  Bi2 O3 . 8_544 2.78(3) ?
  Bi2 O5 . 4_455 2.72(4) ?
  Bi2 O6 . . 2.27(4) ?
  Bi3 O1 . 3_545 3.096(19) ?
  Bi3 O1 . 7_555 2.48(2) ?
  Bi3 O2 . 4_555 2.34(2) ?
  Bi3 O2 . 8_544 2.35(2) ?
  Bi3 O4 . 5_656 2.48(2) ?
  Bi3 O7 . . 2.550(16) ?
  Bi3 O7 . 6_455 2.440(16) ?
  Fe1 Sc1 . . 0 ?
  Fe1 O1 . 1_655 2.00(2) ?
  Fe1 O2 . 6_555 2.08(2) ?
  Fe1 O4 . 3_656 2.17(2) ?
  Fe1 O4 . 8_654 2.01(2) ?
  Fe1 O5 . 2_664 2.080(12) ?
  Fe1 O7 . 7_555 1.974(18) ?
  Sc1 O1 . 1_655 2.00(2) ?
  Sc1 O2 . 6_555 2.08(2) ?
  Sc1 O4 . 3_656 2.17(2) ?
  Sc1 O4 . 8_654 2.01(2) ?
  Sc1 O5 . 2_664 2.080(12) ?
  Sc1 O7 . 7_555 1.974(18) ?
  Fe2 Sc2 . . 0 ?
  Fe2 O1 . 3_645 1.93(2) ?
  Fe2 O2 . 8_544 2.15(2) ?
  Fe2 O3 . 3_646 2.12(3) ?
  Fe2 O3 . 8_644 2.04(3) ?
  Fe2 O6 . . 1.900(12) ?
  Fe2 O7 . . 2.222(18) ?
  Sc2 O1 . 3_645 1.93(2) ?
  Sc2 O2 . 8_544 2.15(2) ?
  Sc2 O3 . 3_646 2.12(3) ?
  Sc2 O3 . 8_644 2.04(3) ?
  Sc2 O6 . . 1.900(12) ?
  Sc2 O7 . . 2.222(18) ?
  O1 O2 . 6_455 2.95(2) ?
  O1 O2 . 6_555 2.77(2) ?
  O1 O4 . 8_554 3.06(3) ?
  O1 O6 . 3_655 2.90(3) ?
  O1 O7 . 3_655 3.04(2) ?
  O1 O7 . 7_455 3.06(2) ?
  O2 O2 . 5_566 2.92(2) ?
  O2 O3 . 6_456 2.81(3) ?
  O2 O4 . 8_554 2.78(3) ?
  O2 O5 . 3_656 2.95(2) ?
  O2 O6 . 2_565 2.91(2) ?
  O2 O7 . 4_455 2.70(2) ?
  O2 O7 . 8_555 2.74(2) ?
  O3 O3 . 6_456 2.85(3) ?
  O3 O3 . 6_556 2.85(3) ?
  O3 O3 . 7_565 2.97(2) ?
  O3 O6 . 2_665 2.93(3) ?
  O3 O6 . 3_656 2.54(3) ?
  O3 O7 . 3_656 3.00(2) ?
  O3 O7 . 8_655 3.05(2) ?
  O4 O4 . 6_456 2.88(2) ?
  O4 O4 . 6_556 2.88(2) ?
  O4 O5 . . 3.01(3) ?
  O4 O5 . 4_456 2.62(3) ?
  O4 O7 . 2_655 2.75(2) ?
  O4 O7 . 5_656 2.74(2) ?
  O5 O6 . 4_555 3.05(4) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  O1 Bi1 O1 2_565 . 8_545 91.3(7) ?
  O1 Bi1 O4 2_565 . 4_456 79.2(6) ?
  O1 Bi1 O4 2_565 . 6_456 163.6(11) ?
  O1 Bi1 O5 2_565 . 1_455 120.2(9) ?
  O1 Bi1 O6 2_565 . 4_455 63.5(7) ?
  O1 Bi1 O4 8_545 . 4_456 163.6(11) ?
  O1 Bi1 O4 8_545 . 6_456 79.2(6) ?
  O1 Bi1 O5 8_545 . 1_455 120.2(9) ?
  O1 Bi1 O6 8_545 . 4_455 63.5(7) ?
  O4 Bi1 O4 4_456 . 6_456 106.4(12) ?
  O4 Bi1 O5 4_456 . 1_455 76.3(9) ?
  O4 Bi1 O6 4_456 . 4_455 122.0(8) ?
  O4 Bi1 O5 6_456 . 1_455 76.3(9) ?
  O4 Bi1 O6 6_456 . 4_455 122.0(8) ?
  O5 Bi1 O6 1_455 . 4_455 85.7(14) ?
  O2 Bi2 O2 2_564 . 8_544 108.8(9) ?
  O2 Bi2 O3 2_564 . 2_564 92.3(5) ?
  O2 Bi2 O3 2_564 . 3_646 131.7(11) ?
  O2 Bi2 O3 2_564 . 5_666 62.3(7) ?
  O2 Bi2 O3 2_564 . 8_544 155.2(8) ?
  O2 Bi2 O5 2_564 . 4_455 60.9(6) ?
  O2 Bi2 O6 2_564 . . 64.2(6) ?
  O2 Bi2 O3 8_544 . 2_564 155.2(8) ?
  O2 Bi2 O3 8_544 . 3_646 62.3(7) ?
  O2 Bi2 O3 8_544 . 5_666 131.7(11) ?
  O2 Bi2 O3 8_544 . 8_544 92.3(5) ?
  O2 Bi2 O5 8_544 . 4_455 60.9(6) ?
  O2 Bi2 O6 8_544 . . 64.2(6) ?
  O3 Bi2 O3 2_564 . 3_646 112.8(12) ?
  O3 Bi2 O3 2_564 . 5_666 69.3(9) ?
  O3 Bi2 O3 2_564 . 8_544 64.5(7) ?
  O3 Bi2 O5 2_564 . 4_455 124.0(9) ?
  O3 Bi2 O6 2_564 . . 139.4(9) ?
  O3 Bi2 O3 3_646 . 5_666 88.1(11) ?
  O3 Bi2 O3 3_646 . 8_544 69.3(9) ?
  O3 Bi2 O5 3_646 . 4_455 121.7(10) ?
  O3 Bi2 O6 3_646 . . 70.4(10) ?
  O3 Bi2 O3 5_666 . 8_544 112.8(12) ?
  O3 Bi2 O5 5_666 . 4_455 121.7(10) ?
  O3 Bi2 O6 5_666 . . 70.4(10) ?
  O3 Bi2 O5 8_544 . 4_455 124.0(9) ?
  O3 Bi2 O6 8_544 . . 139.4(9) ?
  O5 Bi2 O6 4_455 . . 74.8(12) ?
  O1 Bi3 O1 3_545 . 7_555 80.6(6) ?
  O1 Bi3 O2 3_545 . 4_555 112.5(7) ?
  O1 Bi3 O2 3_545 . 8_544 63.8(6) ?
  O1 Bi3 O4 3_545 . 5_656 164.0(6) ?
  O1 Bi3 O7 3_545 . . 129.9(6) ?
  O1 Bi3 O7 3_545 . 6_455 110.9(6) ?
  O1 Bi3 O2 7_555 . 4_555 69.9(6) ?
  O1 Bi3 O2 7_555 . 8_544 115.9(8) ?
  O1 Bi3 O4 7_555 . 5_656 85.9(7) ?
  O1 Bi3 O7 7_555 . . 134.2(6) ?
  O1 Bi3 O7 7_555 . 6_455 117.4(7) ?
  O2 Bi3 O2 4_555 . 8_544 76.9(7) ?
  O2 Bi3 O4 4_555 . 5_656 70.2(7) ?
  O2 Bi3 O7 4_555 . . 66.8(6) ?
  O2 Bi3 O7 4_555 . 6_455 136.6(8) ?
  O2 Bi3 O4 8_544 . 5_656 130.8(8) ?
  O2 Bi3 O7 8_544 . . 67.8(6) ?
  O2 Bi3 O7 8_544 . 6_455 124.4(8) ?
  O4 Bi3 O7 5_656 . . 66.1(6) ?
  O4 Bi3 O7 5_656 . 6_455 67.9(7) ?
  O7 Bi3 O7 . . 6_455 86.0(5) ?
  Sc1 Fe1 O1 . . 1_655 0 ?
  Sc1 Fe1 O2 . . 6_555 0 ?
  Sc1 Fe1 O4 . . 3_656 0 ?
  Sc1 Fe1 O4 . . 8_654 0 ?
  Sc1 Fe1 O5 . . 2_664 0 ?
  Sc1 Fe1 O7 . . 7_555 0 ?
  O1 Fe1 O2 1_655 . 6_555 92.5(9) ?
  O1 Fe1 O4 1_655 . 3_656 172.8(10) ?
  O1 Fe1 O4 1_655 . 8_654 99.3(9) ?
  O1 Fe1 O5 1_655 . 2_664 99.8(10) ?
  O1 Fe1 O7 1_655 . 7_555 100.8(7) ?
  O2 Fe1 O4 6_555 . 3_656 81.6(9) ?
  O2 Fe1 O4 6_555 . 8_654 166.2(10) ?
  O2 Fe1 O5 6_555 . 2_664 90.2(10) ?
  O2 Fe1 O7 6_555 . 7_555 83.4(7) ?
  O4 Fe1 O4 3_656 . 8_654 87.1(9) ?
  O4 Fe1 O5 3_656 . 2_664 76.3(10) ?
  O4 Fe1 O7 3_656 . 7_555 82.7(7) ?
  O4 Fe1 O5 8_654 . 2_664 94.8(11) ?
  O4 Fe1 O7 8_654 . 7_555 87.2(7) ?
  O5 Fe1 O7 2_664 . 7_555 158.7(11) ?
  Fe1 Sc1 O1 . . 1_655 0 ?
  Fe1 Sc1 O2 . . 6_555 0 ?
  Fe1 Sc1 O4 . . 3_656 0 ?
  Fe1 Sc1 O4 . . 8_654 0 ?
  Fe1 Sc1 O5 . . 2_664 0 ?
  Fe1 Sc1 O7 . . 7_555 0 ?
  O1 Sc1 O2 1_655 . 6_555 92.5(9) ?
  O1 Sc1 O4 1_655 . 3_656 172.8(10) ?
  O1 Sc1 O4 1_655 . 8_654 99.3(9) ?
  O1 Sc1 O5 1_655 . 2_664 99.8(10) ?
  O1 Sc1 O7 1_655 . 7_555 100.8(7) ?
  O2 Sc1 O4 6_555 . 3_656 81.6(9) ?
  O2 Sc1 O4 6_555 . 8_654 166.2(10) ?
  O2 Sc1 O5 6_555 . 2_664 90.2(10) ?
  O2 Sc1 O7 6_555 . 7_555 83.4(7) ?
  O4 Sc1 O4 3_656 . 8_654 87.1(9) ?
  O4 Sc1 O5 3_656 . 2_664 76.3(10) ?
  O4 Sc1 O7 3_656 . 7_555 82.7(7) ?
  O4 Sc1 O5 8_654 . 2_664 94.8(11) ?
  O4 Sc1 O7 8_654 . 7_555 87.2(7) ?
  O5 Sc1 O7 2_664 . 7_555 158.7(11) ?
  Sc2 Fe2 O1 . . 3_645 0 ?
  Sc2 Fe2 O2 . . 8_544 0 ?
  Sc2 Fe2 O3 . . 3_646 0 ?
  Sc2 Fe2 O3 . . 8_644 0 ?
  Sc2 Fe2 O6 . . . 0 ?
  Sc2 Fe2 O7 . . . 0 ?
  O1 Fe2 O2 3_645 . 8_544 85.5(8) ?
  O1 Fe2 O3 3_645 . 3_646 167.0(10) ?
  O1 Fe2 O3 3_645 . 8_644 106.8(10) ?
  O1 Fe2 O6 3_645 . . 98.5(12) ?
  O1 Fe2 O7 3_645 . . 93.9(6) ?
  O2 Fe2 O3 8_544 . 3_646 82.1(9) ?
  O2 Fe2 O3 8_544 . 8_644 164.0(10) ?
  O2 Fe2 O6 8_544 . . 91.9(11) ?
  O2 Fe2 O7 8_544 . . 77.6(6) ?
  O3 Fe2 O3 3_646 . 8_644 86.1(10) ?
  O3 Fe2 O6 3_646 . . 78.0(11) ?
  O3 Fe2 O7 3_646 . . 87.3(6) ?
  O3 Fe2 O6 8_644 . . 96.2(11) ?
  O3 Fe2 O7 8_644 . . 91.1(7) ?
  O6 Fe2 O7 . . . 163.1(11) ?
  Fe2 Sc2 O1 . . 3_645 0 ?
  Fe2 Sc2 O2 . . 8_544 0 ?
  Fe2 Sc2 O3 . . 3_646 0 ?
  Fe2 Sc2 O3 . . 8_644 0 ?
  Fe2 Sc2 O6 . . . 0 ?
  Fe2 Sc2 O7 . . . 0 ?
  O1 Sc2 O2 3_645 . 8_544 85.5(8) ?
  O1 Sc2 O3 3_645 . 3_646 167.0(10) ?
  O1 Sc2 O3 3_645 . 8_644 106.8(10) ?
  O1 Sc2 O6 3_645 . . 98.5(12) ?
  O1 Sc2 O7 3_645 . . 93.9(6) ?
  O2 Sc2 O3 8_544 . 3_646 82.1(9) ?
  O2 Sc2 O3 8_544 . 8_644 164.0(10) ?
  O2 Sc2 O6 8_544 . . 91.9(11) ?
  O2 Sc2 O7 8_544 . . 77.6(6) ?
  O3 Sc2 O3 3_646 . 8_644 86.1(10) ?
  O3 Sc2 O6 3_646 . . 78.0(11) ?
  O3 Sc2 O7 3_646 . . 87.3(6) ?
  O3 Sc2 O6 8_644 . . 96.2(11) ?
  O3 Sc2 O7 8_644 . . 91.1(7) ?
  O6 Sc2 O7 . . . 163.1(11) ?
  Bi1 O1 Bi3 2_564 . 3_555 174.2(7) ?
  Bi1 O1 Bi3 2_564 . 7_555 86.4(6) ?
  Bi1 O1 Fe1 2_564 . 1_455 96.1(9) ?
  Bi1 O1 Sc1 2_564 . 1_455 96.1(9) ?
  Bi1 O1 Fe2 2_564 . 3_655 83.2(7) ?
  Bi1 O1 Sc2 2_564 . 3_655 83.2(7) ?
  Bi1 O1 O2 2_564 . 6_455 131.4(7) ?
  Bi1 O1 O2 2_564 . 6_555 64.9(6) ?
  Bi1 O1 O4 2_564 . 8_554 65.8(7) ?
  Bi1 O1 O6 2_564 . 3_655 49.0(8) ?
  Bi1 O1 O7 2_564 . 3_655 118.4(6) ?
  Bi1 O1 O7 2_564 . 7_455 118.8(9) ?
  Bi3 O1 Bi3 3_555 . 7_555 99.4(6) ?
  Bi3 O1 Fe1 3_555 . 1_455 83.8(5) ?
  Bi3 O1 Sc1 3_555 . 1_455 83.8(5) ?
  Bi3 O1 Fe2 3_555 . 3_655 95.0(8) ?
  Bi3 O1 Sc2 3_555 . 3_655 95.0(8) ?
  Bi3 O1 O2 3_555 . 6_455 45.7(5) ?
  Bi3 O1 O2 3_555 . 6_555 118.1(7) ?
  Bi3 O1 O4 3_555 . 8_554 116.7(6) ?
  Bi3 O1 O6 3_555 . 3_655 127.0(10) ?
  Bi3 O1 O7 3_555 . 3_655 63.2(5) ?
  Bi3 O1 O7 3_555 . 7_455 64.4(4) ?
  Bi3 O1 Fe1 7_555 . 1_455 99.0(9) ?
  Bi3 O1 Sc1 7_555 . 1_455 99.0(9) ?
  Bi3 O1 Fe2 7_555 . 3_655 99.0(6) ?
  Bi3 O1 Sc2 7_555 . 3_655 99.0(6) ?
  Bi3 O1 O2 7_555 . 6_455 121.3(7) ?
  Bi3 O1 O2 7_555 . 6_555 52.7(5) ?
  Bi3 O1 O4 7_555 . 8_554 71.4(7) ?
  Bi3 O1 O6 7_555 . 3_655 112.0(7) ?
  Bi3 O1 O7 7_555 . 3_655 72.2(5) ?
  Bi3 O1 O7 7_555 . 7_455 70.0(6) ?
  Fe1 O1 Sc1 1_455 . 1_455 0.0(5) ?
  Fe1 O1 Fe2 1_455 . 3_655 161.9(10) ?
  Fe1 O1 Sc2 1_455 . 3_655 161.9(10) ?
  Fe1 O1 O2 1_455 . 6_455 44.8(6) ?
  Fe1 O1 O2 1_455 . 6_555 144.6(11) ?
  Fe1 O1 O4 1_455 . 8_554 40.5(6) ?
  Fe1 O1 O6 1_455 . 3_655 128.7(8) ?
  Fe1 O1 O7 1_455 . 3_655 143.0(7) ?
  Fe1 O1 O7 1_455 . 7_455 39.3(5) ?
  Sc1 O1 Fe2 1_455 . 3_655 161.9(10) ?
  Sc1 O1 Sc2 1_455 . 3_655 161.9(10) ?
  Sc1 O1 O2 1_455 . 6_455 44.8(6) ?
  Sc1 O1 O2 1_455 . 6_555 144.6(11) ?
  Sc1 O1 O4 1_455 . 8_554 40.5(6) ?
  Sc1 O1 O6 1_455 . 3_655 128.7(8) ?
  Sc1 O1 O7 1_455 . 3_655 143.0(7) ?
  Sc1 O1 O7 1_455 . 7_455 39.3(5) ?
  Fe2 O1 Sc2 3_655 . 3_655 0.0(5) ?
  Fe2 O1 O2 3_655 . 6_455 124.4(11) ?
  Fe2 O1 O2 3_655 . 6_555 50.6(6) ?
  Fe2 O1 O4 3_655 . 8_554 147.7(8) ?
  Fe2 O1 O6 3_655 . 3_655 40.4(6) ?
  Fe2 O1 O7 3_655 . 3_655 46.8(5) ?
  Fe2 O1 O7 3_655 . 7_455 153.4(8) ?
  Sc2 O1 O2 3_655 . 6_455 124.4(11) ?
  Sc2 O1 O2 3_655 . 6_555 50.6(6) ?
  Sc2 O1 O4 3_655 . 8_554 147.7(8) ?
  Sc2 O1 O6 3_655 . 3_655 40.4(6) ?
  Sc2 O1 O7 3_655 . 3_655 46.8(5) ?
  Sc2 O1 O7 3_655 . 7_455 153.4(8) ?
  O2 O1 O2 6_455 . 6_555 163.7(8) ?
  O2 O1 O4 6_455 . 8_554 85.0(7) ?
  O2 O1 O6 6_455 . 3_655 126.7(9) ?
  O2 O1 O7 6_455 . 3_655 108.4(7) ?
  O2 O1 O7 6_455 . 7_455 53.3(5) ?
  O2 O1 O4 6_555 . 8_554 104.8(8) ?
  O2 O1 O6 6_555 . 3_655 61.8(6) ?
  O2 O1 O7 6_555 . 3_655 56.0(5) ?
  O2 O1 O7 6_555 . 7_455 122.6(7) ?
  O4 O1 O6 8_554 . 3_655 113.4(9) ?
  O4 O1 O7 8_554 . 3_655 142.9(7) ?
  O4 O1 O7 8_554 . 7_455 53.4(5) ?
  O6 O1 O7 3_655 . 3_655 86.7(7) ?
  O6 O1 O7 3_655 . 7_455 166.0(10) ?
  O7 O1 O7 3_655 . 7_455 106.8(6) ?
  Bi2 O2 Bi3 2_565 . 4_455 157.8(8) ?
  Bi2 O2 Bi3 2_565 . 8_555 98.6(8) ?
  Bi2 O2 Fe1 2_565 . 6_455 85.5(7) ?
  Bi2 O2 Sc1 2_565 . 6_455 85.5(7) ?
  Bi2 O2 Fe2 2_565 . 8_555 73.3(7) ?
  Bi2 O2 Sc2 2_565 . 8_555 73.3(7) ?
  Bi2 O2 O1 2_565 . 6_455 105.7(7) ?
  Bi2 O2 O1 2_565 . 6_555 66.3(6) ?
  Bi2 O2 O2 2_565 . 5_566 149.8(9) ?
  Bi2 O2 O3 2_565 . 6_456 42.3(6) ?
  Bi2 O2 O4 2_565 . 8_554 107.1(7) ?
  Bi2 O2 O5 2_565 . 3_656 53.8(8) ?
  Bi2 O2 O6 2_565 . 2_565 44.5(7) ?
  Bi2 O2 O7 2_565 . 4_455 128.8(8) ?
  Bi2 O2 O7 2_565 . 8_555 107.7(9) ?
  Bi3 O2 Bi3 4_455 . 8_555 103.1(7) ?
  Bi3 O2 Fe1 4_455 . 6_455 93.4(9) ?
  Bi3 O2 Sc1 4_455 . 6_455 93.4(9) ?
  Bi3 O2 Fe2 4_455 . 8_555 97.3(8) ?
  Bi3 O2 Sc2 4_455 . 8_555 97.3(8) ?
  Bi3 O2 O1 4_455 . 6_455 57.4(6) ?
  Bi3 O2 O1 4_455 . 6_555 125.7(9) ?
  Bi3 O2 O2 4_455 . 5_566 51.7(6) ?
  Bi3 O2 O3 4_455 . 6_456 141.8(9) ?
  Bi3 O2 O4 4_455 . 8_554 57.2(6) ?
  Bi3 O2 O5 4_455 . 3_656 111.4(10) ?
  Bi3 O2 O6 4_455 . 2_565 116.1(9) ?
  Bi3 O2 O7 4_455 . 4_455 60.3(6) ?
  Bi3 O2 O7 4_455 . 8_555 80.1(6) ?
  Bi3 O2 Fe1 8_555 . 6_455 104.3(8) ?
  Bi3 O2 Sc1 8_555 . 6_455 104.3(8) ?
  Bi3 O2 Fe2 8_555 . 8_555 102.8(10) ?
  Bi3 O2 Sc2 8_555 . 8_555 102.8(10) ?
  Bi3 O2 O1 8_555 . 6_455 125.7(9) ?
  Bi3 O2 O1 8_555 . 6_555 70.5(6) ?
  Bi3 O2 O2 8_555 . 5_566 51.5(6) ?
  Bi3 O2 O3 8_555 . 6_456 74.2(8) ?
  Bi3 O2 O4 8_555 . 8_554 140.8(9) ?
  Bi3 O2 O5 8_555 . 3_656 133.2(9) ?
  Bi3 O2 O6 8_555 . 2_565 126.8(11) ?
  Bi3 O2 O7 8_555 . 4_455 80.8(6) ?
  Bi3 O2 O7 8_555 . 8_555 59.5(6) ?
  Fe1 O2 Sc1 6_455 . 6_455 0.0(5) ?
  Fe1 O2 Fe2 6_455 . 8_555 147.7(8) ?
  Fe1 O2 Sc2 6_455 . 8_555 147.7(8) ?
  Fe1 O2 O1 6_455 . 6_455 125.1(10) ?
  Fe1 O2 O1 6_455 . 6_555 42.7(6) ?
  Fe1 O2 O2 6_455 . 5_566 104.2(8) ?
  Fe1 O2 O3 6_455 . 6_456 124.6(9) ?
  Fe1 O2 O4 6_455 . 8_554 50.6(7) ?
  Fe1 O2 O5 6_455 . 3_656 44.9(7) ?
  Fe1 O2 O6 6_455 . 2_565 107.6(8) ?
  Fe1 O2 O7 6_455 . 4_455 46.6(6) ?
  Fe1 O2 O7 6_455 . 8_555 159.9(8) ?
  Sc1 O2 Fe2 6_455 . 8_555 147.7(8) ?
  Sc1 O2 Sc2 6_455 . 8_555 147.7(8) ?
  Sc1 O2 O1 6_455 . 6_455 125.1(10) ?
  Sc1 O2 O1 6_455 . 6_555 42.7(6) ?
  Sc1 O2 O2 6_455 . 5_566 104.2(8) ?
  Sc1 O2 O3 6_455 . 6_456 124.6(9) ?
  Sc1 O2 O4 6_455 . 8_554 50.6(7) ?
  Sc1 O2 O5 6_455 . 3_656 44.9(7) ?
  Sc1 O2 O6 6_455 . 2_565 107.6(8) ?
  Sc1 O2 O7 6_455 . 4_455 46.6(6) ?
  Sc1 O2 O7 6_455 . 8_555 159.9(8) ?
  Fe2 O2 Sc2 8_555 . 8_555 0.0(5) ?
  Fe2 O2 O1 8_555 . 6_455 43.9(6) ?
  Fe2 O2 O1 8_555 . 6_555 137.0(10) ?
  Fe2 O2 O2 8_555 . 5_566 106.3(8) ?
  Fe2 O2 O3 8_555 . 6_456 48.6(7) ?
  Fe2 O2 O4 8_555 . 8_554 112.5(8) ?
  Fe2 O2 O5 8_555 . 3_656 103.0(8) ?
  Fe2 O2 O6 8_555 . 2_565 40.7(6) ?
  Fe2 O2 O7 8_555 . 4_455 157.3(9) ?
  Fe2 O2 O7 8_555 . 8_555 52.4(6) ?
  Sc2 O2 O1 8_555 . 6_455 43.9(6) ?
  Sc2 O2 O1 8_555 . 6_555 137.0(10) ?
  Sc2 O2 O2 8_555 . 5_566 106.3(8) ?
  Sc2 O2 O3 8_555 . 6_456 48.6(7) ?
  Sc2 O2 O4 8_555 . 8_554 112.5(8) ?
  Sc2 O2 O5 8_555 . 3_656 103.0(8) ?
  Sc2 O2 O6 8_555 . 2_565 40.7(6) ?
  Sc2 O2 O7 8_555 . 4_455 157.3(9) ?
  Sc2 O2 O7 8_555 . 8_555 52.4(6) ?
  O1 O2 O1 6_455 . 6_555 163.7(8) ?
  O1 O2 O2 6_455 . 5_566 92.1(6) ?
  O1 O2 O3 6_455 . 6_456 92.5(9) ?
  O1 O2 O4 6_455 . 8_554 75.2(8) ?
  O1 O2 O5 6_455 . 3_656 99.7(8) ?
  O1 O2 O6 6_455 . 2_565 61.3(7) ?
  O1 O2 O7 6_455 . 4_455 116.0(9) ?
  O1 O2 O7 6_455 . 8_555 67.0(6) ?
  O1 O2 O2 6_555 . 5_566 101.5(6) ?
  O1 O2 O3 6_555 . 6_456 90.1(8) ?
  O1 O2 O4 6_555 . 8_554 93.3(8) ?
  O1 O2 O5 6_555 . 3_656 64.0(7) ?
  O1 O2 O6 6_555 . 2_565 108.5(8) ?
  O1 O2 O7 6_555 . 4_455 65.5(6) ?
  O1 O2 O7 6_555 . 8_555 128.3(8) ?
  O2 O2 O3 5_566 . 6_456 114.3(9) ?
  O2 O2 O4 5_566 . 8_554 100.9(8) ?
  O2 O2 O5 5_566 . 3_656 147.7(11) ?
  O2 O2 O6 5_566 . 2_565 146.6(9) ?
  O2 O2 O7 5_566 . 4_455 58.2(6) ?
  O2 O2 O7 5_566 . 8_555 56.9(6) ?
  O3 O2 O4 6_456 . 8_554 143.2(7) ?
  O3 O2 O5 6_456 . 3_656 95.3(8) ?
  O3 O2 O6 6_456 . 2_565 52.7(8) ?
  O3 O2 O7 6_456 . 4_455 149.9(9) ?
  O3 O2 O7 6_456 . 8_555 65.5(7) ?
  O4 O2 O5 8_554 . 3_656 54.5(8) ?
  O4 O2 O6 8_554 . 2_565 91.8(9) ?
  O4 O2 O7 8_554 . 4_455 60.1(6) ?
  O4 O2 O7 8_554 . 8_555 133.9(8) ?
  O5 O2 O6 3_656 . 2_565 62.7(8) ?
  O5 O2 O7 3_656 . 4_455 89.7(9) ?
  O5 O2 O7 3_656 . 8_555 155.0(9) ?
  O6 O2 O7 2_565 . 4_455 149.7(10) ?
  O6 O2 O7 2_565 . 8_555 92.3(9) ?
  O7 O2 O7 4_455 . 8_555 115.1(7) ?
  Bi2 O3 Bi2 2_565 . 3_656 103.0(8) ?
  Bi2 O3 Fe2 2_565 . 3_656 84.6(9) ?
  Bi2 O3 Fe2 2_565 . 8_655 93.5(10) ?
  Bi2 O3 Sc2 2_565 . 3_656 84.6(9) ?
  Bi2 O3 Sc2 2_565 . 8_655 93.5(10) ?
  Bi2 O3 O2 2_565 . 6_556 132.1(10) ?
  Bi2 O3 O3 2_565 . 6_456 44.6(6) ?
  Bi2 O3 O3 2_565 . 6_556 127.1(10) ?
  Bi2 O3 O3 2_565 . 7_565 57.8(6) ?
  Bi2 O3 O6 2_565 . 2_665 75.0(8) ?
  Bi2 O3 O6 2_565 . 3_656 73.4(9) ?
  Bi2 O3 O7 2_565 . 3_656 105.1(8) ?
  Bi2 O3 O7 2_565 . 8_655 122.9(9) ?
  Bi2 O3 Fe2 3_656 . 3_656 97.3(11) ?
  Bi2 O3 Fe2 3_656 . 8_655 106.1(12) ?
  Bi2 O3 Sc2 3_656 . 3_656 97.3(11) ?
  Bi2 O3 Sc2 3_656 . 8_655 106.1(12) ?
  Bi2 O3 O2 3_656 . 6_556 75.4(9) ?
  Bi2 O3 O3 3_656 . 6_456 121.2(11) ?
  Bi2 O3 O3 3_656 . 6_556 66.1(9) ?
  Bi2 O3 O3 3_656 . 7_565 46.0(7) ?
  Bi2 O3 O6 3_656 . 2_665 76.1(10) ?
  Bi2 O3 O6 3_656 . 3_656 57.2(10) ?
  Bi2 O3 O7 3_656 . 3_656 131.2(11) ?
  Bi2 O3 O7 3_656 . 8_655 123.9(11) ?
  Fe2 O3 Fe2 3_656 . 8_655 156.3(11) ?
  Fe2 O3 Sc2 3_656 . 3_656 0.0(5) ?
  Fe2 O3 Sc2 3_656 . 8_655 156.3(11) ?
  Fe2 O3 O2 3_656 . 6_556 49.3(6) ?
  Fe2 O3 O3 3_656 . 6_456 45.7(7) ?
  Fe2 O3 O3 3_656 . 6_556 145.9(11) ?
  Fe2 O3 O3 3_656 . 7_565 99.2(8) ?
  Fe2 O3 O6 3_656 . 2_665 156.3(9) ?
  Fe2 O3 O6 3_656 . 3_656 47.0(6) ?
  Fe2 O3 O7 3_656 . 3_656 47.7(5) ?
  Fe2 O3 O7 3_656 . 8_655 115.8(7) ?
  Fe2 O3 Sc2 8_655 . 3_656 156.3(11) ?
  Fe2 O3 Sc2 8_655 . 8_655 0.0(5) ?
  Fe2 O3 O2 8_655 . 6_556 133.6(10) ?
  Fe2 O3 O3 8_655 . 6_456 120.2(11) ?
  Fe2 O3 O3 8_655 . 6_556 48.2(7) ?
  Fe2 O3 O3 8_655 . 7_565 99.6(9) ?
  Fe2 O3 O6 8_655 . 2_665 40.1(5) ?
  Fe2 O3 O6 8_655 . 3_656 153.9(10) ?
  Fe2 O3 O7 8_655 . 3_656 111.0(7) ?
  Fe2 O3 O7 8_655 . 8_655 46.8(5) ?
  Sc2 O3 Sc2 3_656 . 8_655 156.3(11) ?
  Sc2 O3 O2 3_656 . 6_556 49.3(6) ?
  Sc2 O3 O3 3_656 . 6_456 45.7(7) ?
  Sc2 O3 O3 3_656 . 6_556 145.9(11) ?
  Sc2 O3 O3 3_656 . 7_565 99.2(8) ?
  Sc2 O3 O6 3_656 . 2_665 156.3(9) ?
  Sc2 O3 O6 3_656 . 3_656 47.0(6) ?
  Sc2 O3 O7 3_656 . 3_656 47.7(5) ?
  Sc2 O3 O7 3_656 . 8_655 115.8(7) ?
  Sc2 O3 O2 8_655 . 6_556 133.6(10) ?
  Sc2 O3 O3 8_655 . 6_456 120.2(11) ?
  Sc2 O3 O3 8_655 . 6_556 48.2(7) ?
  Sc2 O3 O3 8_655 . 7_565 99.6(9) ?
  Sc2 O3 O6 8_655 . 2_665 40.1(5) ?
  Sc2 O3 O6 8_655 . 3_656 153.9(10) ?
  Sc2 O3 O7 8_655 . 3_656 111.0(7) ?
  Sc2 O3 O7 8_655 . 8_655 46.8(5) ?
  O2 O3 O3 6_556 . 6_456 94.4(9) ?
  O2 O3 O3 6_556 . 6_556 96.7(9) ?
  O2 O3 O3 6_556 . 7_565 111.1(9) ?
  O2 O3 O6 6_556 . 2_665 144.6(11) ?
  O2 O3 O6 6_556 . 3_656 65.8(8) ?
  O2 O3 O7 6_556 . 3_656 56.2(5) ?
  O2 O3 O7 6_556 . 8_655 92.8(6) ?
  O3 O3 O3 6_456 . 6_556 168.1(11) ?
  O3 O3 O3 6_456 . 7_565 90.0(8) ?
  O3 O3 O6 6_456 . 2_665 118.4(10) ?
  O3 O3 O6 6_456 . 3_656 65.7(9) ?
  O3 O3 O7 6_456 . 3_656 62.7(6) ?
  O3 O3 O7 6_456 . 8_655 114.1(7) ?
  O3 O3 O3 6_556 . 7_565 90.0(8) ?
  O3 O3 O6 6_556 . 2_665 52.1(8) ?
  O3 O3 O6 6_556 . 3_656 123.1(11) ?
  O3 O3 O7 6_556 . 3_656 120.9(7) ?
  O3 O3 O7 6_556 . 8_655 61.1(6) ?
  O3 O3 O6 7_565 . 2_665 59.6(6) ?
  O3 O3 O6 7_565 . 3_656 54.3(7) ?
  O3 O3 O7 7_565 . 3_656 146.2(10) ?
  O3 O3 O7 7_565 . 8_655 145.0(9) ?
  O6 O3 O6 2_665 . 3_656 113.8(8) ?
  O6 O3 O7 2_665 . 3_656 149.9(9) ?
  O6 O3 O7 2_665 . 8_655 86.0(7) ?
  O6 O3 O7 3_656 . 3_656 94.4(8) ?
  O6 O3 O7 3_656 . 8_655 158.2(10) ?
  O7 O3 O7 3_656 . 8_655 68.5(5) ?
  Bi1 O4 Bi3 4_556 . 5_656 106.3(10) ?
  Bi1 O4 Fe1 4_556 . 3_646 92.9(10) ?
  Bi1 O4 Fe1 4_556 . 8_645 112.9(10) ?
  Bi1 O4 Sc1 4_556 . 3_646 92.9(10) ?
  Bi1 O4 Sc1 4_556 . 8_645 112.9(10) ?
  Bi1 O4 O1 4_556 . 8_545 130.9(9) ?
  Bi1 O4 O2 4_556 . 8_545 75.7(9) ?
  Bi1 O4 O4 4_556 . 6_456 112.8(9) ?
  Bi1 O4 O4 4_556 . 6_556 79.0(8) ?
  Bi1 O4 O5 4_556 . . 73.3(9) ?
  Bi1 O4 O5 4_556 . 4_456 48.2(9) ?
  Bi1 O4 O7 4_556 . 2_655 135.9(10) ?
  Bi1 O4 O7 4_556 . 5_656 131.7(11) ?
  Bi3 O4 Fe1 5_656 . 3_646 87.5(8) ?
  Bi3 O4 Fe1 5_656 . 8_645 97.8(8) ?
  Bi3 O4 Sc1 5_656 . 3_646 87.5(8) ?
  Bi3 O4 Sc1 5_656 . 8_645 97.8(8) ?
  Bi3 O4 O1 5_656 . 8_545 116.1(7) ?
  Bi3 O4 O2 5_656 . 8_545 52.6(6) ?
  Bi3 O4 O4 5_656 . 6_456 116.6(8) ?
  Bi3 O4 O4 5_656 . 6_556 74.6(6) ?
  Bi3 O4 O5 5_656 . . 126.9(8) ?
  Bi3 O4 O5 5_656 . 4_456 118.4(11) ?
  Bi3 O4 O7 5_656 . 2_655 55.3(5) ?
  Bi3 O4 O7 5_656 . 5_656 58.2(5) ?
  Fe1 O4 Fe1 3_646 . 8_645 150.7(11) ?
  Fe1 O4 Sc1 3_646 . 3_646 0.0(5) ?
  Fe1 O4 Sc1 3_646 . 8_645 150.7(11) ?
  Fe1 O4 O1 3_646 . 8_545 111.9(8) ?
  Fe1 O4 O2 3_646 . 8_545 47.8(6) ?
  Fe1 O4 O4 3_646 . 6_456 44.2(6) ?
  Fe1 O4 O4 3_646 . 6_556 157.2(11) ?
  Fe1 O4 O5 3_646 . . 145.0(9) ?
  Fe1 O4 O5 3_646 . 4_456 50.3(7) ?
  Fe1 O4 O7 3_646 . 2_655 122.1(8) ?
  Fe1 O4 O7 3_646 . 5_656 45.6(5) ?
  Fe1 O4 Sc1 8_645 . 3_646 150.7(11) ?
  Fe1 O4 Sc1 8_645 . 8_645 0.0(5) ?
  Fe1 O4 O1 8_645 . 8_545 40.3(6) ?
  Fe1 O4 O2 8_645 . 8_545 149.8(9) ?
  Fe1 O4 O4 8_645 . 6_456 109.6(10) ?
  Fe1 O4 O4 8_645 . 6_556 48.7(7) ?
  Fe1 O4 O5 8_645 . . 43.5(6) ?
  Fe1 O4 O5 8_645 . 4_456 141.9(10) ?
  Fe1 O4 O7 8_645 . 2_655 45.8(5) ?
  Fe1 O4 O7 8_645 . 5_656 114.4(8) ?
  Sc1 O4 Sc1 3_646 . 8_645 150.7(11) ?
  Sc1 O4 O1 3_646 . 8_545 111.9(8) ?
  Sc1 O4 O2 3_646 . 8_545 47.8(6) ?
  Sc1 O4 O4 3_646 . 6_456 44.2(6) ?
  Sc1 O4 O4 3_646 . 6_556 157.2(11) ?
  Sc1 O4 O5 3_646 . . 145.0(9) ?
  Sc1 O4 O5 3_646 . 4_456 50.3(7) ?
  Sc1 O4 O7 3_646 . 2_655 122.1(8) ?
  Sc1 O4 O7 3_646 . 5_656 45.6(5) ?
  Sc1 O4 O1 8_645 . 8_545 40.3(6) ?
  Sc1 O4 O2 8_645 . 8_545 149.8(9) ?
  Sc1 O4 O4 8_645 . 6_456 109.6(10) ?
  Sc1 O4 O4 8_645 . 6_556 48.7(7) ?
  Sc1 O4 O5 8_645 . . 43.5(6) ?
  Sc1 O4 O5 8_645 . 4_456 141.9(10) ?
  Sc1 O4 O7 8_645 . 2_655 45.8(5) ?
  Sc1 O4 O7 8_645 . 5_656 114.4(8) ?
  O1 O4 O2 8_545 . 8_545 151.3(8) ?
  O1 O4 O4 8_545 . 6_456 69.4(7) ?
  O1 O4 O4 8_545 . 6_556 89.0(8) ?
  O1 O4 O5 8_545 . . 61.9(7) ?
  O1 O4 O5 8_545 . 4_456 120.4(10) ?
  O1 O4 O7 8_545 . 2_655 63.4(6) ?
  O1 O4 O7 8_545 . 5_656 92.8(6) ?
  O2 O4 O4 8_545 . 6_456 91.6(8) ?
  O2 O4 O4 8_545 . 6_556 109.4(9) ?
  O2 O4 O5 8_545 . . 146.8(10) ?
  O2 O4 O5 8_545 . 4_456 66.0(8) ?
  O2 O4 O7 8_545 . 2_655 107.1(7) ?
  O2 O4 O7 8_545 . 5_656 58.5(6) ?
  O4 O4 O4 6_456 . 6_556 158.2(11) ?
  O4 O4 O5 6_456 . . 111.3(9) ?
  O4 O4 O5 6_456 . 4_456 66.1(8) ?
  O4 O4 O7 6_456 . 2_655 111.0(8) ?
  O4 O4 O7 6_456 . 5_656 58.5(5) ?
  O4 O4 O5 6_556 . . 52.8(7) ?
  O4 O4 O5 6_556 . 4_456 127.1(9) ?
  O4 O4 O7 6_556 . 2_655 58.2(6) ?
  O4 O4 O7 6_556 . 5_656 128.0(7) ?
  O5 O4 O5 . . 4_456 100.7(8) ?
  O5 O4 O7 . . 2_655 87.4(7) ?
  O5 O4 O7 . . 5_656 154.4(10) ?
  O5 O4 O7 4_456 . 2_655 172.0(10) ?
  O5 O4 O7 4_456 . 5_656 95.8(8) ?
  O7 O4 O7 2_655 . 5_656 76.6(6) ?
  Bi1 O5 Bi2 1_655 . 4_555 98.9(15) ?
  Bi1 O5 Fe1 1_655 . 2_665 102.2(8) ?
  Bi1 O5 Fe1 1_655 . 8_645 102.2(8) ?
  Bi1 O5 Sc1 1_655 . 2_665 102.2(8) ?
  Bi1 O5 Sc1 1_655 . 8_645 102.2(8) ?
  Bi1 O5 O2 1_655 . 3_646 74.7(8) ?
  Bi1 O5 O2 1_655 . 5_666 74.7(8) ?
  Bi1 O5 O4 1_655 . . 114.9(12) ?
  Bi1 O5 O4 1_655 . 4_556 55.5(8) ?
  Bi1 O5 O4 1_655 . 6_556 55.5(8) ?
  Bi1 O5 O4 1_655 . 7_555 114.9(12) ?
  Bi1 O5 O6 1_655 . 4_555 53.1(11) ?
  Bi2 O5 Fe1 4_555 . 2_665 95.0(10) ?
  Bi2 O5 Fe1 4_555 . 8_645 95.0(10) ?
  Bi2 O5 Sc1 4_555 . 2_665 95.0(10) ?
  Bi2 O5 Sc1 4_555 . 8_645 95.0(10) ?
  Bi2 O5 O2 4_555 . 3_646 65.4(8) ?
  Bi2 O5 O2 4_555 . 5_666 65.4(8) ?
  Bi2 O5 O4 4_555 . . 127.9(9) ?
  Bi2 O5 O4 4_555 . 4_556 123.3(10) ?
  Bi2 O5 O4 4_555 . 6_556 123.3(10) ?
  Bi2 O5 O4 4_555 . 7_555 127.9(9) ?
  Bi2 O5 O6 4_555 . 4_555 45.8(9) ?
  Fe1 O5 Fe1 2_665 . 8_645 151.8(16) ?
  Fe1 O5 Sc1 2_665 . 2_665 0.0(5) ?
  Fe1 O5 Sc1 2_665 . 8_645 151.8(16) ?
  Fe1 O5 O2 2_665 . 3_646 158.9(16) ?
  Fe1 O5 O2 2_665 . 5_666 44.9(6) ?
  Fe1 O5 O4 2_665 . . 113.7(13) ?
  Fe1 O5 O4 2_665 . 4_556 53.4(6) ?
  Fe1 O5 O4 2_665 . 6_556 136.2(15) ?
  Fe1 O5 O4 2_665 . 7_555 41.7(7) ?
  Fe1 O5 O6 2_665 . 4_555 103.0(9) ?
  Fe1 O5 Sc1 8_645 . 2_665 151.8(16) ?
  Fe1 O5 Sc1 8_645 . 8_645 0.0(5) ?
  Fe1 O5 O2 8_645 . 3_646 44.9(6) ?
  Fe1 O5 O2 8_645 . 5_666 158.9(16) ?
  Fe1 O5 O4 8_645 . . 41.7(7) ?
  Fe1 O5 O4 8_645 . 4_556 136.2(15) ?
  Fe1 O5 O4 8_645 . 6_556 53.4(6) ?
  Fe1 O5 O4 8_645 . 7_555 113.7(13) ?
  Fe1 O5 O6 8_645 . 4_555 103.0(9) ?
  Sc1 O5 Sc1 2_665 . 8_645 151.8(16) ?
  Sc1 O5 O2 2_665 . 3_646 158.9(16) ?
  Sc1 O5 O2 2_665 . 5_666 44.9(6) ?
  Sc1 O5 O4 2_665 . . 113.7(13) ?
  Sc1 O5 O4 2_665 . 4_556 53.4(6) ?
  Sc1 O5 O4 2_665 . 6_556 136.2(15) ?
  Sc1 O5 O4 2_665 . 7_555 41.7(7) ?
  Sc1 O5 O6 2_665 . 4_555 103.0(9) ?
  Sc1 O5 O2 8_645 . 3_646 44.9(6) ?
  Sc1 O5 O2 8_645 . 5_666 158.9(16) ?
  Sc1 O5 O4 8_645 . . 41.7(7) ?
  Sc1 O5 O4 8_645 . 4_556 136.2(15) ?
  Sc1 O5 O4 8_645 . 6_556 53.4(6) ?
  Sc1 O5 O4 8_645 . 7_555 113.7(13) ?
  Sc1 O5 O6 8_645 . 4_555 103.0(9) ?
  O2 O5 O2 3_646 . 5_666 115.6(12) ?
  O2 O5 O4 3_646 . . 85.9(5) ?
  O2 O5 O4 3_646 . 4_556 129.9(11) ?
  O2 O5 O4 3_646 . 6_556 59.5(7) ?
  O2 O5 O4 3_646 . 7_555 158.5(10) ?
  O2 O5 O6 3_646 . 4_555 58.1(6) ?
  O2 O5 O4 5_666 . . 158.5(10) ?
  O2 O5 O4 5_666 . 4_556 59.5(7) ?
  O2 O5 O4 5_666 . 6_556 129.9(11) ?
  O2 O5 O4 5_666 . 7_555 85.9(5) ?
  O2 O5 O6 5_666 . 4_555 58.1(6) ?
  O4 O5 O4 . . 4_556 108.7(13) ?
  O4 O5 O4 . . 6_556 61.0(7) ?
  O4 O5 O4 . . 7_555 72.6(9) ?
  O4 O5 O6 . . 4_555 143.4(5) ?
  O4 O5 O4 4_556 . 6_556 85.6(11) ?
  O4 O5 O4 4_556 . 7_555 61.0(7) ?
  O4 O5 O6 4_556 . 4_555 91.9(10) ?
  O4 O5 O4 6_556 . 7_555 108.7(13) ?
  O4 O5 O6 6_556 . 4_555 91.9(10) ?
  O4 O5 O6 7_555 . 4_555 143.4(5) ?
  Bi1 O6 Bi2 4_555 . . 100.6(14) ?
  Bi1 O6 Fe2 4_555 . . 100.7(11) ?
  Bi1 O6 Fe2 4_555 . 7_555 100.7(11) ?
  Bi1 O6 Sc2 4_555 . . 100.7(11) ?
  Bi1 O6 Sc2 4_555 . 7_555 100.7(11) ?
  Bi1 O6 O1 4_555 . 3_645 67.5(9) ?
  Bi1 O6 O1 4_555 . 5_665 67.5(9) ?
  Bi1 O6 O2 4_555 . 2_564 70.1(8) ?
  Bi1 O6 O2 4_555 . 8_544 70.1(8) ?
  Bi1 O6 O3 4_555 . 2_664 133.2(11) ?
  Bi1 O6 O3 4_555 . 3_646 129.6(11) ?
  Bi1 O6 O3 4_555 . 5_666 129.6(11) ?
  Bi1 O6 O3 4_555 . 8_644 133.2(11) ?
  Bi1 O6 O5 4_555 . 4_455 41.2(9) ?
  Bi2 O6 Fe2 . . . 99.8(10) ?
  Bi2 O6 Fe2 . . 7_555 99.8(10) ?
  Bi2 O6 Sc2 . . . 99.8(10) ?
  Bi2 O6 Sc2 . . 7_555 99.8(10) ?
  Bi2 O6 O1 . . 3_645 128.0(7) ?
  Bi2 O6 O1 . . 5_665 128.0(7) ?
  Bi2 O6 O2 . . 2_564 71.3(7) ?
  Bi2 O6 O2 . . 8_544 71.3(7) ?
  Bi2 O6 O3 . . 2_664 113.0(13) ?
  Bi2 O6 O3 . . 3_646 52.3(9) ?
  Bi2 O6 O3 . . 5_666 52.3(9) ?
  Bi2 O6 O3 . . 8_644 113.0(13) ?
  Bi2 O6 O5 . . 4_455 59.4(11) ?
  Fe2 O6 Fe2 . . 7_555 147.5(18) ?
  Fe2 O6 Sc2 . . . 0.0(5) ?
  Fe2 O6 Sc2 . . 7_555 147.5(18) ?
  Fe2 O6 O1 . . 3_645 41.1(7) ?
  Fe2 O6 O1 . . 5_665 131.7(14) ?
  Fe2 O6 O2 . . 2_564 165.1(15) ?
  Fe2 O6 O2 . . 8_544 47.4(6) ?
  Fe2 O6 O3 . . 2_664 104.4(13) ?
  Fe2 O6 O3 . . 3_646 54.9(8) ?
  Fe2 O6 O3 . . 5_666 123.1(16) ?
  Fe2 O6 O3 . . 8_644 43.7(8) ?
  Fe2 O6 O5 . . 4_455 106.1(10) ?
  Fe2 O6 Sc2 7_555 . . 147.5(18) ?
  Fe2 O6 Sc2 7_555 . 7_555 0.0(5) ?
  Fe2 O6 O1 7_555 . 3_645 131.7(14) ?
  Fe2 O6 O1 7_555 . 5_665 41.1(7) ?
  Fe2 O6 O2 7_555 . 2_564 47.4(6) ?
  Fe2 O6 O2 7_555 . 8_544 165.1(15) ?
  Fe2 O6 O3 7_555 . 2_664 43.7(8) ?
  Fe2 O6 O3 7_555 . 3_646 123.1(16) ?
  Fe2 O6 O3 7_555 . 5_666 54.9(8) ?
  Fe2 O6 O3 7_555 . 8_644 104.4(13) ?
  Fe2 O6 O5 7_555 . 4_455 106.1(10) ?
  Sc2 O6 Sc2 . . 7_555 147.5(18) ?
  Sc2 O6 O1 . . 3_645 41.1(7) ?
  Sc2 O6 O1 . . 5_665 131.7(14) ?
  Sc2 O6 O2 . . 2_564 165.1(15) ?
  Sc2 O6 O2 . . 8_544 47.4(6) ?
  Sc2 O6 O3 . . 2_664 104.4(13) ?
  Sc2 O6 O3 . . 3_646 54.9(8) ?
  Sc2 O6 O3 . . 5_666 123.1(16) ?
  Sc2 O6 O3 . . 8_644 43.7(8) ?
  Sc2 O6 O5 . . 4_455 106.1(10) ?
  Sc2 O6 O1 7_555 . 3_645 131.7(14) ?
  Sc2 O6 O1 7_555 . 5_665 41.1(7) ?
  Sc2 O6 O2 7_555 . 2_564 47.4(6) ?
  Sc2 O6 O2 7_555 . 8_544 165.1(15) ?
  Sc2 O6 O3 7_555 . 2_664 43.7(8) ?
  Sc2 O6 O3 7_555 . 3_646 123.1(16) ?
  Sc2 O6 O3 7_555 . 5_666 54.9(8) ?
  Sc2 O6 O3 7_555 . 8_644 104.4(13) ?
  Sc2 O6 O5 7_555 . 4_455 106.1(10) ?
  O1 O6 O1 3_645 . 5_665 95.3(10) ?
  O1 O6 O2 3_645 . 2_564 135.9(14) ?
  O1 O6 O2 3_645 . 8_544 56.9(5) ?
  O1 O6 O3 3_645 . 2_664 110.1(10) ?
  O1 O6 O3 3_645 . 3_646 95.2(6) ?
  O1 O6 O3 3_645 . 5_666 162.5(14) ?
  O1 O6 O3 3_645 . 8_644 66.2(7) ?
  O1 O6 O5 3_645 . 4_455 94.5(10) ?
  O1 O6 O2 5_665 . 2_564 56.9(5) ?
  O1 O6 O2 5_665 . 8_544 135.9(14) ?
  O1 O6 O3 5_665 . 2_664 66.2(7) ?
  O1 O6 O3 5_665 . 3_646 162.5(14) ?
  O1 O6 O3 5_665 . 5_666 95.2(6) ?
  O1 O6 O3 5_665 . 8_644 110.1(10) ?
  O1 O6 O5 5_665 . 4_455 94.5(10) ?
  O2 O6 O2 2_564 . 8_544 117.7(12) ?
  O2 O6 O3 2_564 . 2_664 90.3(6) ?
  O2 O6 O3 2_564 . 3_646 121.4(12) ?
  O2 O6 O3 2_564 . 5_666 61.4(7) ?
  O2 O6 O3 2_564 . 8_644 150.5(11) ?
  O2 O6 O5 2_564 . 4_455 59.2(7) ?
  O2 O6 O3 8_544 . 2_664 150.5(11) ?
  O2 O6 O3 8_544 . 3_646 61.4(7) ?
  O2 O6 O3 8_544 . 5_666 121.4(12) ?
  O2 O6 O3 8_544 . 8_644 90.3(6) ?
  O2 O6 O5 8_544 . 4_455 59.2(7) ?
  O3 O6 O3 2_664 . 3_646 97.1(13) ?
  O3 O6 O3 2_664 . 5_666 62.1(9) ?
  O3 O6 O3 2_664 . 8_644 60.7(8) ?
  O3 O6 O5 2_664 . 4_455 149.4(5) ?
  O3 O6 O3 3_646 . 5_666 71.5(10) ?
  O3 O6 O3 3_646 . 8_644 62.1(9) ?
  O3 O6 O5 3_646 . 4_455 98.6(11) ?
  O3 O6 O3 5_666 . 8_644 97.1(13) ?
  O3 O6 O5 5_666 . 4_455 98.6(11) ?
  O3 O6 O5 8_644 . 4_455 149.4(5) ?
  Bi3 O7 Bi3 . . 6_555 109.6(6) ?
  Bi3 O7 Fe1 . . 7_555 90.0(6) ?
  Bi3 O7 Sc1 . . 7_555 90.0(6) ?
  Bi3 O7 Fe2 . . . 94.7(6) ?
  Bi3 O7 Sc2 . . . 94.7(6) ?
  Bi3 O7 O1 . . 3_645 109.1(6) ?
  Bi3 O7 O1 . . 7_655 114.1(6) ?
  Bi3 O7 O2 . . 4_555 53.0(5) ?
  Bi3 O7 O2 . . 8_544 52.7(5) ?
  Bi3 O7 O3 . . 3_646 68.1(6) ?
  Bi3 O7 O3 . . 8_644 124.1(7) ?
  Bi3 O7 O4 . . 2_654 119.0(7) ?
  Bi3 O7 O4 . . 5_656 55.7(5) ?
  Bi3 O7 Fe1 6_555 . 7_555 100.1(7) ?
  Bi3 O7 Sc1 6_555 . 7_555 100.1(7) ?
  Bi3 O7 Fe2 6_555 . . 106.5(7) ?
  Bi3 O7 Sc2 6_555 . . 106.5(7) ?
  Bi3 O7 O1 6_555 . 3_645 129.5(7) ?
  Bi3 O7 O1 6_555 . 7_655 117.1(7) ?
  Bi3 O7 O2 6_555 . 4_555 138.7(8) ?
  Bi3 O7 O2 6_555 . 8_544 139.7(8) ?
  Bi3 O7 O3 6_555 . 3_646 81.8(6) ?
  Bi3 O7 O3 6_555 . 8_644 68.6(6) ?
  Bi3 O7 O4 6_555 . 2_654 56.7(6) ?
  Bi3 O7 O4 6_555 . 5_656 77.9(6) ?
  Fe1 O7 Sc1 7_555 . 7_555 0.0(5) ?
  Fe1 O7 Fe2 7_555 . . 149.7(7) ?
  Fe1 O7 Sc2 7_555 . . 149.7(7) ?
  Fe1 O7 O1 7_555 . 3_645 111.2(6) ?
  Fe1 O7 O1 7_555 . 7_655 40.0(5) ?
  Fe1 O7 O2 7_555 . 4_555 49.9(6) ?
  Fe1 O7 O2 7_555 . 8_544 114.2(7) ?
  Fe1 O7 O3 7_555 . 3_646 157.0(8) ?
  Fe1 O7 O3 7_555 . 8_644 145.9(7) ?
  Fe1 O7 O4 7_555 . 2_654 46.9(6) ?
  Fe1 O7 O4 7_555 . 5_656 51.7(6) ?
  Sc1 O7 Fe2 7_555 . . 149.7(7) ?
  Sc1 O7 Sc2 7_555 . . 149.7(7) ?
  Sc1 O7 O1 7_555 . 3_645 111.2(6) ?
  Sc1 O7 O1 7_555 . 7_655 40.0(5) ?
  Sc1 O7 O2 7_555 . 4_555 49.9(6) ?
  Sc1 O7 O2 7_555 . 8_544 114.2(7) ?
  Sc1 O7 O3 7_555 . 3_646 157.0(8) ?
  Sc1 O7 O3 7_555 . 8_644 145.9(7) ?
  Sc1 O7 O4 7_555 . 2_654 46.9(6) ?
  Sc1 O7 O4 7_555 . 5_656 51.7(6) ?
  Fe2 O7 Sc2 . . . 0.0(5) ?
  Fe2 O7 O1 . . 3_645 39.3(5) ?
  Fe2 O7 O1 . . 7_655 112.4(6) ?
  Fe2 O7 O2 . . 4_555 111.7(7) ?
  Fe2 O7 O2 . . 8_544 49.9(5) ?
  Fe2 O7 O3 . . 3_646 45.0(6) ?
  Fe2 O7 O3 . . 8_644 42.1(5) ?
  Fe2 O7 O4 . . 2_654 145.3(7) ?
  Fe2 O7 O4 . . 5_656 148.6(7) ?
  Sc2 O7 O1 . . 3_645 39.3(5) ?
  Sc2 O7 O1 . . 7_655 112.4(6) ?
  Sc2 O7 O2 . . 4_555 111.7(7) ?
  Sc2 O7 O2 . . 8_544 49.9(5) ?
  Sc2 O7 O3 . . 3_646 45.0(6) ?
  Sc2 O7 O3 . . 8_644 42.1(5) ?
  Sc2 O7 O4 . . 2_654 145.3(7) ?
  Sc2 O7 O4 . . 5_656 148.6(7) ?
  O1 O7 O1 3_645 . 7_655 73.2(5) ?
  O1 O7 O2 3_645 . 4_555 91.0(6) ?
  O1 O7 O2 3_645 . 8_544 57.0(5) ?
  O1 O7 O3 3_645 . 3_646 83.6(6) ?
  O1 O7 O3 3_645 . 8_644 63.2(6) ?
  O1 O7 O4 3_645 . 2_654 124.4(6) ?
  O1 O7 O4 3_645 . 5_656 152.4(8) ?
  O1 O7 O2 7_655 . 4_555 61.2(5) ?
  O1 O7 O2 7_655 . 8_544 102.9(7) ?
  O1 O7 O3 7_655 . 3_646 156.2(7) ?
  O1 O7 O3 7_655 . 8_644 115.1(6) ?
  O1 O7 O4 7_655 . 2_654 63.2(7) ?
  O1 O7 O4 7_655 . 5_656 91.5(6) ?
  O2 O7 O2 4_555 . 8_544 64.9(6) ?
  O2 O7 O3 4_555 . 3_646 115.0(7) ?
  O2 O7 O3 4_555 . 8_644 152.5(8) ?
  O2 O7 O4 4_555 . 2_654 96.4(7) ?
  O2 O7 O4 4_555 . 5_656 61.4(7) ?
  O2 O7 O3 8_544 . 3_646 58.3(7) ?
  O2 O7 O3 8_544 . 8_644 91.4(7) ?
  O2 O7 O4 8_544 . 2_654 161.1(8) ?
  O2 O7 O4 8_544 . 5_656 106.6(6) ?
  O3 O7 O3 3_646 . 8_644 56.2(6) ?
  O3 O7 O4 3_646 . 2_654 138.3(8) ?
  O3 O7 O4 3_646 . 5_656 107.3(7) ?
  O3 O7 O4 8_644 . 2_654 105.9(7) ?
  O3 O7 O4 8_644 . 5_656 143.9(8) ?
  O4 O7 O4 2_654 . 5_656 63.3(6) ?
 
loop_
_geom_torsion_atom_site_label_1 
_geom_torsion_atom_site_label_2 
_geom_torsion_atom_site_label_3 
_geom_torsion_atom_site_label_4 
_geom_torsion_site_symmetry_1   
_geom_torsion_site_symmetry_2   
_geom_torsion_site_symmetry_3   
_geom_torsion_site_symmetry_4   
_geom_torsion                   
_geom_torsion_publ_flag         
?   ?   ?   ?   ?   ?   ?   ?   ?   ?
 
loop_
_geom_hbond_atom_site_label_D 
_geom_hbond_atom_site_label_H 
_geom_hbond_atom_site_label_A 
_geom_hbond_site_symmetry_D   
_geom_hbond_site_symmetry_H   
_geom_hbond_site_symmetry_A   
_geom_hbond_distance_DH       
_geom_hbond_distance_HA       
_geom_hbond_distance_DA       
_geom_hbond_angle_DHA         
_geom_hbond_publ_flag         
?   ?   ?   ?   ?   ?   ?   ?   ?   ?   ?
 
#=============================================================================
 
#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
